Please fill this form, we will try to respond as soon as possible.

March 6, 2007ACI E702 Example Problems Acceptance of Concrete Test Results L.M. Snell Title: Acceptance of concrete test results according to the American Concrete Institute’s, ACI 318-05, Building Code Requirements for Structural Concrete. Problem: You are the Field Engineer on a project that is currently underway. The project specification states that the concrete strength is 3500 psi in twenty-eight (28) days. The following data contains the two (2) twenty eight (28) day cylinder test data that was sent to you by the testing laboratory. You need to evaluate this data and determine if the concrete is acceptable. Test # 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 Assumptions 1. Sampling frequency is adequate; the minimal frequency is: a. Once a day for a given class b. Once every 150 yards³ c. Once each 5000 feet² of surface area for slabs or walls (ACI 318.5.6.2.1) 2. Samples are taken on a random basis – concrete was not to be sampled due to appearance, convenience, or other biased criteria. (ACI 318.5.6.2.2 and ACI 318R. 5.6.2.2) 3. Each set of cylinders come from a different batch of concrete. (ACI 318.5.6.2.2 and ACI 318R 5.6.2.2) 4. No water was added to the concrete after the samples were taken. (ACI 318R. 5.6.2.2) 5. Qualified field testing technicians performed the test on the fresh concrete. (ACI 318.5.6.1) 6. Qualified laboratory technician performed all required laboratory tests. (ACI 318.5.6.1) Cylinder #1 (psi) 4100 4320 4310 4420 4200 4250 3880 3570 3570 3780 3680 3300 3470 2770 3200 Cylinder #2 (psi) 4320 4190 4310 4380 4160 3810 4040 3680 3210 3780 2980 3740 3210 2750 3480 1 2007 ACI E702 Example Problems Acceptance of Concrete Test Results L. Determine the arithmetic average of any three (3) consecutive strength test results. Snell Solution 1.M.5.6.March 6.4) Cylinder 1 + Cylinder 2 = strength test results 2 On our project: For strength test #1: 4100 + 4320 = 4210 psi 2 Thus the strength test results are: Test # 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 Strength Test Results (psi) 4210 4255 4310 4400 4180 4030 3960 3625 3390 3780 3330 3520 3340 2760 3340 2. (ACI 318.3. (ACI 318.5.3a) For the first three (3) strength test results – ST1 + ST2 + ST3 = Arithmetic Average 3 2 .2. Determine the strength test results (average strength of two tests cylinders from the same batch and tested at 28 days or at test age designed for determination of f’c.6. M. This does not indicate a problem since the strength test result is 3390 psi. inspect the strength test results for: f’c – 500 or 3500 – 500 = 3000 psi On our project: Strength test result # 14 is the only strength test result below 3000 psi.March 6. 2007 ACI E702 Example Problems Acceptance of Concrete Test Results L. The strength test result is 3330 psi.3b) Since f’c = 3500 psi.6. this is above 3000 psi. • 3 . Notes: • Only the strength test results (average of 2 cylinders) are to be used not the individual cylinders results. the concrete is acceptable.3. Snell On our project 4210 + 4255 + 4310 = 4258 psi 3 Thus. the arithmetic averages are: Test # 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 Arithmetic Average (psi) ------------4258 4322 4297 4203 4057 3872 3658 3598 3500 3543 3397 3207 3147 3. this is above 3000 psi. (ACI 318. thus. Test # 11 has a cylinder test result of 2980 psi. • Test # 9 has one cylinder test result below 3500 psi (3210 psi).10f’c when f’c is more than 5000 psi. thus the concrete is acceptable. Determine if any strength test results are below f’c – 500 or by more than 0.5. including strict compliance with standard test procedures (ACI 318R.6.4) On our project Changes need to be made so that we do not continue to make questionable concrete. b. steps must be taken to improve the strength of future concrete placements. 4 . Reductions in or better control of levels of slump supplied d. we must improve future concrete placement. The arithmetic average of three (3) are below f’c (3500 psi) on test numbers 13. Closer control of air content f.3. (ACI 318. 5. The concrete in this area does not meet the strength criteria and needs to be evaluated.6.4) On our project: a.M. An improvement in the quality of the testing.3. Determine if either the arithmetic average (calculated in Step 2) is below f’c or if the strength test result is f’c – 500 psi (calculated in 3). 6. If the strength test result is below f’c – 500. Options of what needs to be done: a. Thus on our project. An increase in cementitious materials content b. 5. Snell 4.5.5.6. steps must be taken to assure that the load carrying capacity of the structure is not jeopardized (ACI 318.5. Change in mixture proportions c. A reduction in delivery time e.1) On our project: Concrete placed at the location identified by test number 14 is below f’c – 500 or 3000 psi. and 15. 14. 2007 ACI E702 Example Problems Acceptance of Concrete Test Results L. One or more of the above needs to be implemented once the problem(s) of why we are having low strength tests is identified.March 6. Strength test results below f’c – 500 or 3000 psi occurs at test number 14. 6.2R – Nondestructive Test Methods for Evaluation of Concrete Structures ACI 301 – Specifications for Structural Concrete ACI 437 – Strength Evaluation of Existing Concrete Buildings 5 . a.5. If further investigation is deemed necessary. and structural adequacy remains in doubt.6. How to determine what needs to be done to assure that the load carrying capacity is not jeopardized.5. Are there other documents other than ACI 318 that can help me with additional analysis on testing data? ACI have several documents which may be used.5) d.5.6. These include: • • • • • ACI 214 – Evaluation of Strength Test Results of Concrete ACI 228. Snell 7. The average strength of the cores must exceed 85% of 3500 psi or 2975 psi and b. How to determine if cores indicate that the concrete is acceptable Concrete is considered structurally adequate if the average of the three (3) cores equals or exceeds 85% of f’c and no single core is less than 75% of f’c.M. No single core strength is below 75% of 3500 psi or 2625 psi. 2007 ACI E702 Example Problems Acceptance of Concrete Test Results L.6.3) 10.2) 8. consider the test procedures outlined in Chapter 20.4) 9.5.5.1R – In Place Methods to Estimate Concrete Strength ACI 228.5. If these test cores fail.5. a. consider non-destructive testing (ACI 318R. Apply judgment as to the significance of the low test result (ACI 318R.6.March 6.5.6.5) c. (ACI 318. (ACI 318.5.5. Core area(s) of the concrete where load carrying capacity is significantly reduced in accordance with ASTM C 42 (ACI 318.4) On our Project: If we take three (3) cores in the area where the concrete at test location number 14 was placed. Note: Additional core testing is permitted if the core test results are considered erratic. (ACI.